3D model (JSmol)
CompTox Dashboard (EPA)
|Molar mass||172.115 g/mol|
|Appearance||white or pale yellow solid,|
|Melting point||2,400 °C (4,350 °F; 2,670 K)|
|Boiling point||3,500 °C (6,330 °F; 3,770 K)|
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|what is ?)(|
Cerium(IV) oxide, also known as ceric oxide, ceric dioxide, ceria, cerium oxide or cerium dioxide, is an oxide of the rare-earth metal cerium. It is a pale yellow-white powder with the chemical formula CeO2. It is an important commercial product and an intermediate in the purification of the element from the ores. The distinctive property of this material is its reversible conversion to a nonstoichiometric oxide.
Cerium occurs naturally as a mixture with other rare-earth elements in its principal ores bastnaesite and monazite. After extraction of the metal ions into aqueous base, Ce is separated from that mixture by addition of an oxidant followed by adjustment of the pH. This step exploits the low solubility of CeO2 and the fact that other rare-earth elements resist oxidation.
Structure and defect behavior
Cerium oxide adopts the fluorite structure, space group Fm3m, #225 containing 8-coordinate Ce4+ and 4-coordinate O2−. At high temperatures it releases oxygen to give a non-stoichiometric, anion deficient form that retains the fluorite lattice . This material has the formula CeO(2−x), where 0 < x < 0.28. The value of x depends on both the temperature, surface termination and the oxygen partial pressure. The equation
has been shown to predict the equilibrium non stoichiometry x over a wide range of oxygen partial pressures (103–10−4 Pa) and temperatures (1000–1900 °C).
The non stoichiometric form has a blue to black color, and exhibits both ionic and electronic conduction with ionic being the most significant at temperatures > 500 °C.
The number of oxygen vacancies is frequently measured by using X-ray photoelectron spectroscopy to compare the ratios of Ce3+
The primary defects of concern are oxygen vacancies and small polarons (electrons localized on cerium cations). Increasing the concentration of oxygen defects increases the diffusion rate of oxide anions in the lattice as reflected in an increase in ionic conductivity. These factors give ceria favourable performance in applications as a solid electrolyte in solid-oxide fuel cells. Undoped and doped ceria also exhibit high electronic conductivity at low partial pressures of oxygen due to reduction of the cerium ion leading to the formation of small polarons. Since the oxygen atoms in a ceria crystal occur in planes, diffusion of these anions is facile. The diffusion rate increases as the defect concentration increases.
The presence of oxygen vacancies at terminating ceria planes governs the energetics of ceria interactions with adsorbate molecules, and its wettability. Controlling such surface interactions is key to harnessing ceria in catalytic applications. 
Catalysis and surface activity
The primary emerging application of applied CeO2 materials is in the field of catalysis. Surfaces of ceria, in its most stable fluorite phase, are dominated by the lower energy (111) planes, which tend to exhibit lower surface energy. The reaction most commonly catalysed by cerium(IV) is the water gas shift reaction, involving the oxidation of carbon monoxide. Ceria has been explored towards the catalysis of various hydrocarbon conversion reactions including CO2 methanation and the catalytic oxidation of hydrocarbons such as toluene. 
The surface functionality of CeO2 stems largely from its intrinsic hydrophobicity, a trait that is common among rare earth oxides. Hydrophobicity tends to impart resistance to water-deactivation at the surfaces of catalysts and thus enhances the adsorption of organic compounds. Hydrophobicity, which can be conversely seen as organophilicity, is generally associated with higher catalytic performance and is desired in applications involving organic compounds and selective synthesis. 
The interconvertibility of CeOx materials is the basis of the use of ceria for an oxidation catalyst. One small but illustrative use is its use in the walls of self-cleaning ovens as a hydrocarbon oxidation catalyst during the high-temperature cleaning process. Another small scale but famous example is its role in oxidation of natural gas in gas mantles.
Building on its distinct surface interactions, ceria finds further use as a sensor in catalytic converters in automotive applications, controlling the air-exhaust ratio to reduce NOx and carbon monoxide.
The principal industrial application of ceria is for polishing, especially chemical-mechanical planarization (CMP). For this purpose, it has displaced many other oxides that were previously used, such as iron oxide and zirconia. For hobbyists, it is also known as "opticians' rouge".
CeO2 is used to decolorize glass by converting green-tinted ferrous impurities to nearly colorless ferric oxides.
Ceria is of interest as a material for solid oxide fuel cells (SOFCs) because of its relatively high oxygen ion conductivity (i.e. oxygen atoms readily move through it) at intermediate temperatures (500–650 °C) and lower association enthalpy compared to Zirconia system.
Nanoceria has attracted attention as a biological antioxidant.
- Pradyot Patnaik. Handbook of Inorganic Chemicals. McGraw-Hill, 2002, ISBN 0-07-049439-8
- Klaus Reinhardt and Herwig Winkler (2000), "Cerium Mischmetal, Cerium Alloys, and Cerium Compounds", Ullmann's Encyclopedia of Industrial Chemistry, Weinheim: Wiley-VCH, doi:10.1002/14356007.a06_139CS1 maint: Uses authors parameter (link).
- "Standard Thermodynamic Properties of Chemical Substances" (PDF). Archived from the original (PDF) on October 29, 2013.
- DFT study of Cerium Oxide Surfaces Applied surface science 2019 vol 478
- Defects and Defect Processes in Nonmetallic Solids By William Hayes, A. M. Stoneham Courier Dover Publications, 2004.
- Bulfin, B.; Lowe, A. J.; Keogh, K. A.; Murphy, B. E.; Lübben, O.; Krasnikov, S. A.; Shvets, I. V. (2013). "Analytical Model of CeO2 Oxidation and Reduction". The Journal of Physical Chemistry C. 117 (46): 24129–24137. doi:10.1021/jp406578z. hdl:2262/76279.
- Ghillanyova, K.; Galusek, D. (2011). "Chapter 1: Ceramic oxides". In Riedel, Ralf; Chen, I-Wie (eds.). Ceramics Science and Technology, Materials and Properties, vol 2. John Wiley & Sons. ISBN 978-3-527-31156-9.
- Munnings, C.; Badwal, S.P.S.; Fini, D. (2014). "Spontaneous stress-induced oxidation of Ce ions in Gd-doped ceria at room temperature". Ionics. 20 (8): 1117–1126. doi:10.1007/s11581-014-1079-2.
- Badwal, S.P.S.; Daniel Fini; Fabio Ciacchi; Christopher Munnings; Justin Kimpton; John Drennan (2013). "Structural and microstructural stability of ceria – gadolinia electrolyte exposed to reducing environments of high temperature fuel cells". J. Mater. Chem. A. 1 (36): 10768–10782. doi:10.1039/C3TA11752A.
- Hydrophobicity of low-index CeO2 surfaces
- Ruosi Peng; et a. (2018). "Size effect of Pt nanoparticles on the catalytic oxidation of toluene over Pt/CeO2 catalysts". Applied Catalysis B: Environmental. 220.
- Montini, Tiziano; Melchionna, Michele; Monai, Matteo; Fornasiero, Paolo (2016). "Fundamentals and Catalytic Applications of CeO2-Based Materials". Chemical Reviews. 116: 5987���6041. doi:10.1021/acs.chemrev.5b00603.CS1 maint: Uses authors parameter (link)
- By Paier, Joachim; Penschke, Christopher; Sauer, Joachim (2013). "Oxygen Defects and Surface Chemistry of Ceria: Quantum Chemical Studies Compared to Experiment". Chemical Reviews. 113: 3949–3985. doi:10.1021/cr3004949.CS1 maint: Uses authors parameter (link)
- Greenwood, Norman N.; Earnshaw, Alan (1997). Chemistry of the Elements (2nd ed.). Butterworth-Heinemann. ISBN 978-0-08-037941-8.
- Twigg, Martyn V. (2011). "Catalytic control of emissions from cars". Catalysis Today. 163: 33–41. doi:10.1016/j.cattod.2010.12.044.
- Properties of Common Abrasives (Boston Museum of Fine Arts)
- MFA Materials database.
- "Cerium dioxide". DaNa. Archived from the original on 2013-03-02.
- "Mixed conductors". Max Planck institute for solid state research. Retrieved 16 September 2016.
- Arachi, Y. (June 1999). "Electrical conductivity of the ZrO2–Ln2O3 (Ln=lanthanides) system". Solid State Ionics. 121 (1–4): 133–139. doi:10.1016/S0167-2738(98)00540-2.
- "Hydrogen production from solar thermochemical water splitting cycles". SolarPACES. Archived from the original on August 30, 2009.
- Karakoti, A. S.; Monteiro-Riviere, N. A.; Aggarwal, R.; Davis, J. P.; Narayan, R. J.; Self, W. T.; McGinnis, J.; Seal, S. (2008). "Nanoceria as antioxidant: synthesis and biomedical applications". JOM. 60: 33–37. doi:10.1007/s11837-008-0029-8.CS1 maint: Uses authors parameter (link)
|Wikimedia Commons has media related to Cerium(IV) oxide.|